#------------------------------------------------------------------------------
#$Date: 2019-11-17 08:56:31 +0200 (Sun, 17 Nov 2019) $
#$Revision: 228975 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/13/7231396.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7231396
loop_
_publ_author_name
'Luo, Yu-Hui'
'Yi, Li-Qiang'
'Lu, Jia-Ni'
'Dong, Long-Zhang'
'Lan, Ya-Qian'
_publ_section_title
;
 A stable polyoxometalate-based porous coordination polymer with high
 proton conductivity
;
_journal_issue                   39
_journal_name_full               CrystEngComm
_journal_page_first              6077
_journal_paper_doi               10.1039/C8CE00693H
_journal_volume                  20
_journal_year                    2018
_chemical_formula_sum            'C20 H52 Cu4 N12 O60 Si W12'
_chemical_formula_weight         3909.18
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_block_doi                 10.5517/ccdc.csd.cc1z5y7b
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2018-06-25 deposited with the CCDC.
2018-08-14 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 104.296(6)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   13.407(6)
_cell_length_b                   20.998(9)
_cell_length_c                   13.171(6)
_cell_measurement_reflns_used    7682
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.884
_cell_measurement_theta_min      2.156
_cell_volume                     3593(3)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  w/scan
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_unetI/netI     0.0873
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_number            6333
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.014
_diffrn_reflns_theta_max         25.014
_diffrn_reflns_theta_min         1.843
_exptl_absorpt_coefficient_mu    20.410
_exptl_absorpt_correction_T_max  0.294
_exptl_absorpt_correction_T_min  0.154
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    3.613
_exptl_crystal_description       block
_exptl_crystal_F_000             3508
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.06
_refine_diff_density_max         3.072
_refine_diff_density_min         -2.550
_refine_diff_density_rms         0.512
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.035
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     493
_refine_ls_number_reflns         6333
_refine_ls_number_restraints     150
_refine_ls_restrained_S_all      1.030
_refine_ls_R_factor_all          0.1333
_refine_ls_R_factor_gt           0.0802
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0625P)²+451.3654P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1763
_refine_ls_wR_factor_ref         0.1984
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4249
_reflns_number_total             6333
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c8ce00693h2.cif
_cod_data_source_block           mo_lan_0ma
_cod_depositor_comments          'Adding full bibliography for 7231396.cif.'
_cod_database_code               7231396
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.36894(10) 0.37005(6) 0.35863(9) 0.0290(3) Uani 1 1 d . . . . .
W2 W 0.50197(10) 0.47739(6) 0.23470(9) 0.0319(3) Uani 1 1 d . . . . .
W3 W 0.36849(10) 0.39153(6) 0.62266(10) 0.0316(3) Uani 1 1 d . . . . .
W4 W 0.36039(11) 0.60385(6) 0.30538(10) 0.0387(4) Uani 1 1 d . . . . .
W5 W 0.22941(10) 0.49652(7) 0.43022(10) 0.0363(3) Uani 1 1 d . . . . .
W6 W 0.63956(11) 0.37243(6) 0.43038(10) 0.0369(4) Uani 1 1 d . . . . .
Si1 Si 0.5000 0.5000 0.5000 0.0136(19) Uani 1 2 d S U P . .
Cu1 Cu 0.0096(3) 0.2670(2) 0.7811(3) 0.0375(9) Uani 1 1 d . . . . .
Cu2 Cu 0.0087(3) 0.2719(3) 1.0322(3) 0.0589(14) Uani 1 1 d . . . . .
C1 C 0.231(2) 0.3001(14) 0.885(2) 0.027(6) Uani 1 1 d . . . . .
H1 H 0.2538 0.3052 0.8243 0.032 Uiso 1 1 calc R U . . .
C2 C 0.234(2) 0.2917(18) 1.046(2) 0.046(9) Uani 1 1 d . . . . .
H2 H 0.2543 0.2882 1.1190 0.055 Uiso 1 1 calc R U . . .
C3 C 0.455(2) 0.2871(13) 1.111(2) 0.031(7) Uani 1 1 d . . . . .
H3 H 0.4166 0.2751 1.1574 0.037 Uiso 1 1 calc R U . . .
C4 C 0.562(2) 0.2830(14) 1.140(2) 0.032(7) Uani 1 1 d . U . . .
H4 H 0.5966 0.2659 1.2043 0.039 Uiso 1 1 calc R U . . .
C5 C 0.614(2) 0.3049(13) 1.071(2) 0.024(6) Uani 1 1 d . U . . .
C6 C 0.566(2) 0.328(2) 0.974(3) 0.057(12) Uani 1 1 d . . . . .
H6 H 0.6045 0.3409 0.9280 0.069 Uiso 1 1 calc R U . . .
C7 C 0.461(3) 0.3317(19) 0.947(3) 0.052(10) Uani 1 1 d . . . . .
H7 H 0.4274 0.3496 0.8828 0.062 Uiso 1 1 calc R U . . .
C8 C 0.788(2) 0.2761(14) 1.189(2) 0.032(7) Uani 1 1 d . . . . .
H8 H 0.7679 0.2716 1.2511 0.038 Uiso 1 1 calc R U . . .
C9 C 0.791(2) 0.2976(15) 1.028(2) 0.035(7) Uani 1 1 d . U . . .
H9 H 0.7727 0.3103 0.9578 0.041 Uiso 1 1 calc R U . . .
C10 C 0.408(2) 0.3091(13) 1.013(2) 0.029(7) Uani 1 1 d . U . . .
N1 N 0.137(2) 0.2898(13) 0.885(2) 0.038(6) Uani 1 1 d . U . . .
N2 N 0.1380(19) 0.2859(16) 0.9887(19) 0.048(8) Uani 1 1 d . . . . .
N3 N 0.2974(17) 0.3029(11) 0.9857(18) 0.026(5) Uani 1 1 d . U . . .
N4 N 0.879(2) 0.2789(15) 1.0792(19) 0.042(7) Uani 1 1 d . . . . .
N5 N 0.8773(17) 0.2652(13) 1.1779(18) 0.031(6) Uani 1 1 d . . . . .
N6 N 0.7261(19) 0.2955(12) 1.0957(18) 0.032(6) Uani 1 1 d . . . . .
O1 O 0.408(3) 0.4574(18) 0.483(3) 0.029(9) Uani 0.5 1 d . U P A -1
O2 O 0.506(3) 0.5532(17) 0.588(3) 0.033(10) Uani 0.5 1 d . . P A -1
O3 O 0.608(3) 0.4542(18) 0.534(3) 0.025(9) Uani 0.5 1 d . . P A -1
O4 O 0.503(3) 0.5358(16) 0.392(3) 0.020(8) Uani 0.5 1 d . U P A -1
O5 O 0.497(2) 0.6373(13) 0.329(2) 0.068(7) Uani 1 1 d . U . . .
O6 O 0.398(2) 0.5417(13) 0.223(2) 0.070(8) Uani 1 1 d . U . . .
O7 O 0.260(2) 0.5475(14) 0.327(2) 0.078(8) Uani 1 1 d . U . . .
O8 O 0.2981(18) 0.6531(10) 0.2142(16) 0.042(5) Uani 1 1 d . . . . .
O9 O 0.259(2) 0.4272(12) 0.351(2) 0.063(7) Uani 1 1 d . U . . .
O10 O 0.253(2) 0.5673(15) 0.520(2) 0.082(9) Uani 1 1 d . U . . .
O11 O 0.257(2) 0.4421(13) 0.5497(18) 0.069(9) Uani 1 1 d . . . . .
O12 O 0.102(2) 0.4944(14) 0.398(2) 0.069(8) Uani 1 1 d . . . . .
O13 O 0.364(2) 0.3494(13) 0.497(2) 0.065(7) Uani 1 1 d . U . . .
O14 O 0.3074(19) 0.3391(11) 0.6835(19) 0.053(6) Uani 1 1 d . U . . .
O15 O 0.3964(18) 0.4567(13) 0.722(3) 0.084(10) Uani 1 1 d . . . . .
O16 O 0.311(2) 0.3078(11) 0.2916(18) 0.056(7) Uani 1 1 d . . . . .
O17 O 0.5035(19) 0.3395(13) 0.396(2) 0.060(7) Uani 1 1 d . U . . .
O18 O 0.4029(19) 0.4155(12) 0.251(2) 0.057(7) Uani 1 1 d . U . . .
O19 O 0.649(2) 0.3525(15) 0.570(2) 0.079(9) Uani 1 1 d . U . . .
O20 O 0.705(2) 0.3126(10) 0.395(2) 0.055(7) Uani 1 1 d . . . . .
O21 O 0.6036(19) 0.4185(13) 0.302(2) 0.070(9) Uani 1 1 d . . . . .
O22 O 0.505(2) 0.4667(14) 0.1127(19) 0.061(7) Uani 1 1 d . . . . .
O23 O -0.0641(17) 0.2772(11) 0.8864(17) 0.046(6) Uani 1 1 d . U . . .
O24 O 0.078(2) 0.2599(17) 0.6695(19) 0.083(11) Uani 1 1 d . . . . .
O1W O 0.049(4) 0.153(3) 0.826(5) 0.071(13) Uani 0.5 1 d . U P . .
O2W O -0.014(5) 0.379(3) 0.731(5) 0.078(17) Uani 0.5 1 d . U P . .
O3W O -0.027(5) 0.145(3) 0.998(5) 0.082(13) Uani 0.5 1 d . U P . .
O4W O 0.031(5) 0.389(3) 1.091(6) 0.10(2) Uani 0.5 1 d . U P . .
O5W O 0.195(4) 0.462(3) 0.094(4) 0.163(19) Uani 1 1 d . . . . .
O6W O 0.298(4) 0.464(4) 0.939(5) 0.10(2) Uani 0.5 1 d . . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O16 W1 O18 99.9(12) . .
O16 W1 O17 99.8(13) . .
O18 W1 O17 88.7(11) . .
O16 W1 O9 102.2(13) . .
O18 W1 O9 88.1(11) . .
O17 W1 O9 158.0(12) . .
O16 W1 O13 102.0(12) . .
O18 W1 O13 158.0(12) . .
O17 W1 O13 85.8(11) . .
O9 W1 O13 89.1(11) . .
O16 W1 O1 161.4(13) . .
O18 W1 O1 94.1(12) . .
O17 W1 O1 92.5(12) . .
O9 W1 O1 66.0(12) . .
O13 W1 O1 64.9(13) . .
O22 W2 O21 100.7(13) . .
O22 W2 O18 101.9(13) . .
O21 W2 O18 86.6(11) . .
O22 W2 O6 102.1(13) . .
O21 W2 O6 157.2(13) . .
O18 W2 O6 88.6(12) . .
O22 W2 O15 101.8(15) . 3_666
O21 W2 O15 87.5(12) . 3_666
O18 W2 O15 156.3(14) . 3_666
O6 W2 O15 88.0(11) . 3_666
O22 W2 O4 157.2(12) . .
O21 W2 O4 94.4(12) . .
O18 W2 O4 95.9(12) . .
O6 W2 O4 63.9(12) . .
O15 W2 O4 61.7(13) 3_666 .
O14 W3 O5 99.7(13) . 3_666
O14 W3 O15 100.5(13) . .
O5 W3 O15 89.3(11) 3_666 .
O14 W3 O13 101.5(12) . .
O5 W3 O13 88.2(11) 3_666 .
O15 W3 O13 158.0(14) . .
O14 W3 O11 101.1(13) . .
O5 W3 O11 159.2(13) 3_666 .
O15 W3 O11 86.6(12) . .
O13 W3 O11 88.0(10) . .
O14 W3 O1 160.2(13) . .
O5 W3 O1 93.9(13) 3_666 .
O15 W3 O1 93.9(14) . .
O13 W3 O1 64.5(12) . .
O11 W3 O1 66.1(12) . .
O8 W4 O6 100.2(12) . .
O8 W4 O7 104.8(13) . .
O6 W4 O7 87.5(13) . .
O8 W4 O19 101.2(12) . 3_666
O6 W4 O19 158.5(13) . 3_666
O7 W4 O19 88.0(13) . 3_666
O8 W4 O5 100.3(12) . .
O6 W4 O5 88.0(12) . .
O7 W4 O5 154.8(13) . .
O19 W4 O5 87.2(12) 3_666 .
O8 W4 O4 155.3(11) . .
O6 W4 O4 64.2(12) . .
O7 W4 O4 93.9(13) . .
O19 W4 O4 95.2(12) 3_666 .
O5 W4 O4 62.0(12) . .
O12 W5 O7 103.4(13) . .
O12 W5 O10 100.6(14) . .
O7 W5 O10 88.3(13) . .
O12 W5 O9 100.5(13) . .
O7 W5 O9 85.8(12) . .
O10 W5 O9 158.8(13) . .
O12 W5 O11 99.9(13) . .
O7 W5 O11 156.7(14) . .
O10 W5 O11 89.2(13) . .
O9 W5 O11 88.3(11) . .
O12 W5 O1 158.9(14) . .
O7 W5 O1 91.3(14) . .
O10 W5 O1 94.8(13) . .
O9 W5 O1 65.1(12) . .
O11 W5 O1 65.8(12) . .
O20 W6 O19 101.0(13) . .
O20 W6 O17 101.5(12) . .
O19 W6 O17 88.8(12) . .
O20 W6 O21 100.1(12) . .
O19 W6 O21 158.9(13) . .
O17 W6 O21 87.6(11) . .
O20 W6 O10 101.2(13) . 3_666
O19 W6 O10 87.0(13) . 3_666
O17 W6 O10 157.3(13) . 3_666
O21 W6 O10 88.3(13) . 3_666
O20 W6 O3 156.6(13) . .
O19 W6 O3 63.8(13) . .
O17 W6 O3 96.0(12) . .
O21 W6 O3 95.9(13) . .
O10 W6 O3 62.2(13) 3_666 .
O1 Si1 O2 115(2) . .
O1 Si1 O4 110.2(19) . .
O2 Si1 O4 107.6(18) . .
O1 Si1 O3 108.5(19) . .
O2 Si1 O3 108.4(19) . .
O4 Si1 O3 106.9(17) . .
O23 Cu1 O24 176.7(12) . .
O23 Cu1 N1 89.0(10) . .
O24 Cu1 N1 93.1(11) . .
O23 Cu1 N5 90.0(9) . 4_465
O24 Cu1 N5 88.1(10) . 4_465
N1 Cu1 N5 174.7(11) . 4_465
O23 Cu1 O2W 91.9(17) . .
O24 Cu1 O2W 85.5(19) . .
N1 Cu1 O2W 89.4(17) . .
N5 Cu1 O2W 95.9(16) 4_465 .
O23 Cu1 O1W 93.1(15) . .
O24 Cu1 O1W 89.5(17) . .
N1 Cu1 O1W 88.4(16) . .
N5 Cu1 O1W 86.4(16) 4_465 .
O2W Cu1 O1W 174(2) . .
O23 Cu2 O24 163.1(14) . 4_566
O23 Cu2 N2 88.1(10) . .
O24 Cu2 N2 93.9(11) 4_566 .
O23 Cu2 N4 92.3(10) . 1_455
O24 Cu2 N4 89.4(11) 4_566 1_455
N2 Cu2 N4 167.1(14) . 1_455
O23 Cu2 O4W 103.8(19) . .
O24 Cu2 O4W 93(2) 4_566 .
N2 Cu2 O4W 84.4(18) . .
N4 Cu2 O4W 83.0(17) 1_455 .
O23 Cu2 O3W 82.3(15) . .
O24 Cu2 O3W 81.0(17) 4_566 .
N2 Cu2 O3W 103.1(17) . .
N4 Cu2 O3W 89.7(16) 1_455 .
O4W Cu2 O3W 171(2) . .
N1 C1 N3 114(2) . .
N1 C1 H1 123.2 . .
N3 C1 H1 123.2 . .
N3 C2 N2 110(3) . .
N3 C2 H2 124.9 . .
N2 C2 H2 124.9 . .
C10 C3 C4 119(3) . .
C10 C3 H3 120.5 . .
C4 C3 H3 120.5 . .
C5 C4 C3 117(3) . .
C5 C4 H4 121.3 . .
C3 C4 H4 121.3 . .
C4 C5 C6 123(3) . .
C4 C5 N6 118(2) . .
C6 C5 N6 118(2) . .
C7 C6 C5 119(3) . .
C7 C6 H6 120.4 . .
C5 C6 H6 120.4 . .
C10 C7 C6 119(3) . .
C10 C7 H7 120.5 . .
C6 C7 H7 120.5 . .
N5 C8 N6 110(2) . .
N5 C8 H8 125.2 . .
N6 C8 H8 125.2 . .
N4 C9 N6 107(3) . .
N4 C9 H9 126.5 . .
N6 C9 H9 126.5 . .
C7 C10 C3 122(3) . .
C7 C10 N3 123(3) . .
C3 C10 N3 114(2) . .
C1 N1 N2 104(2) . .
C1 N1 Cu1 137(2) . .
N2 N1 Cu1 118.2(19) . .
C2 N2 N1 109(2) . .
C2 N2 Cu2 130(2) . .
N1 N2 Cu2 120.6(19) . .
C2 N3 C1 102(2) . .
C2 N3 C10 130(2) . .
C1 N3 C10 128(2) . .
C9 N4 N5 110(2) . .
C9 N4 Cu2 129(2) . 1_655
N5 N4 Cu2 121(2) . 1_655
C8 N5 N4 109(2) . .
C8 N5 Cu1 132(2) . 4_666
N4 N5 Cu1 119.3(18) . 4_666
C8 N6 C9 105(2) . .
C8 N6 C5 127(2) . .
C9 N6 C5 128(2) . .
Si1 O1 W1 126(2) . .
Si1 O1 W3 123(2) . .
W1 O1 W3 91.6(13) . .
Si1 O1 W5 123(2) . .
W1 O1 W5 91.5(13) . .
W3 O1 W5 91.3(12) . .
Si1 O3 W6 122.3(18) . .
Si1 O4 W2 121.6(18) . .
Si1 O4 W4 120.0(17) . .
W2 O4 W4 93.4(12) . .
W3 O5 W4 138.1(16) 3_666 .
W4 O6 W2 138.4(16) . .
W5 O7 W4 141.2(18) . .
W1 O9 W5 136.7(16) . .
W5 O10 W6 137.5(18) . 3_666
W3 O11 W5 136.5(14) . .
W3 O13 W1 138.3(16) . .
W3 O15 W2 137.7(18) . 3_666
W1 O17 W6 138.5(15) . .
W1 O18 W2 138.4(15) . .
W6 O19 W4 137.6(18) . 3_666
W2 O21 W6 138.3(14) . .
Cu1 O23 Cu2 119.5(11) . .
Cu1 O24 Cu2 122.0(14) . 4_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O16 1.66(2) .
W1 O18 1.85(2) .
W1 O17 1.86(3) .
W1 O9 1.89(2) .
W1 O13 1.89(3) .
W1 O1 2.43(4) .
W2 O22 1.63(2) .
W2 O21 1.89(2) .
W2 O18 1.91(2) .
W2 O6 1.92(3) .
W2 O15 1.93(2) 3_666
W2 O4 2.41(3) .
W3 O14 1.688(19) .
W3 O5 1.86(3) 3_666
W3 O15 1.87(3) .
W3 O13 1.87(3) .
W3 O11 1.89(2) .
W3 O1 2.46(4) .
W4 O8 1.65(2) .
W4 O6 1.85(3) .
W4 O7 1.87(3) .
W4 O19 1.91(3) 3_666
W4 O5 1.91(3) .
W4 O4 2.43(3) .
W5 O12 1.66(3) .
W5 O7 1.85(3) .
W5 O10 1.88(3) .
W5 O9 1.89(3) .
W5 O11 1.90(2) .
W5 O1 2.47(4) .
W6 O20 1.66(2) .
W6 O19 1.86(3) .
W6 O17 1.90(3) .
W6 O21 1.90(3) .
W6 O10 1.91(3) 3_666
W6 O3 2.30(3) .
Si1 O1 1.49(4) .
Si1 O2 1.59(4) .
Si1 O4 1.62(3) .
Si1 O3 1.70(3) .
Cu1 O23 1.90(2) .
Cu1 O24 1.92(2) .
Cu1 N1 1.97(3) .
Cu1 N5 2.06(2) 4_465
Cu1 O2W 2.44(5) .
Cu1 O1W 2.49(5) .
Cu2 O23 1.93(2) .
Cu2 O24 1.94(2) 4_566
Cu2 N2 1.98(3) .
Cu2 N4 1.99(2) 1_455
Cu2 O4W 2.57(7) .
Cu2 O3W 2.73(6) .
C1 N1 1.28(4) .
C1 N3 1.40(3) .
C1 H1 0.9300 .
C2 N3 1.32(4) .
C2 N2 1.33(4) .
C2 H2 0.9300 .
C3 C10 1.37(4) .
C3 C4 1.39(4) .
C3 H3 0.9300 .
C4 C5 1.35(4) .
C4 H4 0.9300 .
C5 C6 1.37(4) .
C5 N6 1.47(3) .
C6 C7 1.36(4) .
C6 H6 0.9300 .
C7 C10 1.35(4) .
C7 H7 0.9300 .
C8 N5 1.26(4) .
C8 N6 1.37(4) .
C8 H8 0.9300 .
C9 N4 1.28(4) .
C9 N6 1.39(4) .
C9 H9 0.9300 .
C10 N3 1.44(4) .
N1 N2 1.36(3) .
N4 N5 1.34(3) .
N4 Cu2 1.99(2) 1_655
N5 Cu1 2.06(2) 4_666
O5 W3 1.86(3) 3_666
O10 W6 1.91(3) 3_666
O15 W2 1.93(2) 3_666
O19 W4 1.91(3) 3_666
O24 Cu2 1.94(2) 4_565
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
C10 C3 C4 C5 4(4) . .
C3 C4 C5 C6 -3(5) . .
C3 C4 C5 N6 -174(3) . .
C4 C5 C6 C7 3(6) . .
N6 C5 C6 C7 174(3) . .
C5 C6 C7 C10 -4(6) . .
C6 C7 C10 C3 5(6) . .
C6 C7 C10 N3 -171(3) . .
C4 C3 C10 C7 -5(5) . .
C4 C3 C10 N3 172(2) . .
N3 C1 N1 N2 1(3) . .
N3 C1 N1 Cu1 -168(2) . .
N3 C2 N2 N1 4(4) . .
N3 C2 N2 Cu2 -178(2) . .
C1 N1 N2 C2 -2(4) . .
Cu1 N1 N2 C2 169(2) . .
C1 N1 N2 Cu2 179(2) . .
Cu1 N1 N2 Cu2 -10(3) . .
N2 C2 N3 C1 -3(4) . .
N2 C2 N3 C10 -177(3) . .
N1 C1 N3 C2 2(3) . .
N1 C1 N3 C10 175(3) . .
C7 C10 N3 C2 -168(4) . .
C3 C10 N3 C2 15(4) . .
C7 C10 N3 C1 20(5) . .
C3 C10 N3 C1 -157(3) . .
N6 C9 N4 N5 -1(4) . .
N6 C9 N4 Cu2 -179(2) . 1_655
N6 C8 N5 N4 2(4) . .
N6 C8 N5 Cu1 -178(2) . 4_666
C9 N4 N5 C8 -1(4) . .
Cu2 N4 N5 C8 177(2) 1_655 .
C9 N4 N5 Cu1 180(2) . 4_666
Cu2 N4 N5 Cu1 -2(3) 1_655 4_666
N5 C8 N6 C9 -3(3) . .
N5 C8 N6 C5 171(3) . .
N4 C9 N6 C8 2(3) . .
N4 C9 N6 C5 -172(3) . .
C4 C5 N6 C8 -12(4) . .
C6 C5 N6 C8 177(3) . .
C4 C5 N6 C9 161(3) . .
C6 C5 N6 C9 -11(5) . .
O2 Si1 O1 W1 -180(2) . .
O4 Si1 O1 W1 59(3) . .
O3 Si1 O1 W1 -58(3) . .
O2 Si1 O1 W3 -59(3) . .
O4 Si1 O1 W3 179.7(18) . .
O3 Si1 O1 W3 63(2) . .
O2 Si1 O1 W5 59(3) . .
O4 Si1 O1 W5 -63(3) . .
O3 Si1 O1 W5 -179.3(19) . .
O1 Si1 O3 W6 57(3) . .
O2 Si1 O3 W6 -178(2) . .
O4 Si1 O3 W6 -62(3) . .
O1 Si1 O4 W2 -56(2) . .
O2 Si1 O4 W2 178(2) . .
O3 Si1 O4 W2 61(2) . .
O1 Si1 O4 W4 59(2) . .
O2 Si1 O4 W4 -67(2) . .
O3 Si1 O4 W4 177.2(18) . .
O8 W4 O6 W2 156(2) . .
O7 W4 O6 W2 -100(3) . .
O19 W4 O6 W2 -22(5) 3_666 .
O5 W4 O6 W2 55(3) . .
O4 W4 O6 W2 -4(2) . .
O12 W5 O7 W4 151(3) . .
O10 W5 O7 W4 51(3) . .
O9 W5 O7 W4 -109(3) . .
O11 W5 O7 W4 -33(5) . .
O1 W5 O7 W4 -44(3) . .
O8 W4 O7 W5 -152(3) . .
O6 W4 O7 W5 108(3) . .
O19 W4 O7 W5 -51(3) 3_666 .
O5 W4 O7 W5 29(5) . .
O4 W4 O7 W5 45(3) . .
O16 W1 O9 W5 156(2) . .
O18 W1 O9 W5 -105(2) . .
O17 W1 O9 W5 -23(4) . .
O13 W1 O9 W5 54(2) . .
O1 W1 O9 W5 -9(2) . .
O12 W5 O9 W1 -155(2) . .
O7 W5 O9 W1 103(2) . .
O10 W5 O9 W1 28(5) . .
O11 W5 O9 W1 -55(2) . .
O1 W5 O9 W1 9.1(19) . .
O12 W5 O10 W6 -157(2) . 3_666
O7 W5 O10 W6 -54(3) . 3_666
O9 W5 O10 W6 20(5) . 3_666
O11 W5 O10 W6 103(3) . 3_666
O1 W5 O10 W6 37(3) . 3_666
O14 W3 O11 W5 -158(2) . .
O5 W3 O11 W5 23(5) 3_666 .
O15 W3 O11 W5 102(2) . .
O13 W3 O11 W5 -56(2) . .
O1 W3 O11 W5 6(2) . .
O14 W3 O13 W1 156(2) . .
O5 W3 O13 W1 -104(2) 3_666 .
O15 W3 O13 W1 -21(4) . .
O11 W3 O13 W1 55(2) . .
O1 W3 O13 W1 -9(2) . .
O16 W1 O13 W3 -157(2) . .
O18 W1 O13 W3 28(4) . .
O17 W1 O13 W3 104(2) . .
O9 W1 O13 W3 -54(2) . .
O1 W1 O13 W3 9(2) . .
O14 W3 O15 W2 152(2) . 3_666
O5 W3 O15 W2 52(3) 3_666 3_666
O13 W3 O15 W2 -31(5) . 3_666
O11 W3 O15 W2 -108(3) . 3_666
O1 W3 O15 W2 -42(3) . 3_666
O16 W1 O17 W6 153(2) . .
O18 W1 O17 W6 53(2) . .
O9 W1 O17 W6 -28(4) . .
O13 W1 O17 W6 -105(2) . .
O1 W1 O17 W6 -41(2) . .
O20 W6 O17 W1 -153(2) . .
O19 W6 O17 W1 106(2) . .
O21 W6 O17 W1 -53(2) . .
O10 W6 O17 W1 27(4) 3_666 .
O3 W6 O17 W1 43(2) . .
O16 W1 O18 W2 -155(2) . .
O17 W1 O18 W2 -56(2) . .
O9 W1 O18 W2 102(2) . .
O13 W1 O18 W2 20(4) . .
O1 W1 O18 W2 37(2) . .
O20 W6 O19 W4 158(2) . 3_666
O17 W6 O19 W4 -101(3) . 3_666
O21 W6 O19 W4 -21(5) . 3_666
O10 W6 O19 W4 57(3) 3_666 3_666
O3 W6 O19 W4 -3(2) . 3_666
O22 W2 O21 W6 -157(3) . .
O18 W2 O21 W6 -56(3) . .
O6 W2 O21 W6 22(5) . .
O15 W2 O21 W6 101(3) 3_666 .
O4 W2 O21 W6 40(3) . .
O20 W6 O21 W2 156(3) . .
O19 W6 O21 W2 -25(5) . .
O17 W6 O21 W2 55(3) . .
O10 W6 O21 W2 -103(3) 3_666 .
O3 W6 O21 W2 -41(3) . .
